#------------------------------------------------------------------------------
#$Date: 2023-03-16 05:03:16 +0200 (Thu, 16 Mar 2023) $
#$Revision: 281906 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/90/2109099.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2109099
loop_
_publ_author_name
'Yakubovich, Olga V.'
'Kiriukhina, Galina V.'
'Simonov, Sergey V.'
'Volkov, Anatoly S.'
'Dimitrova, Olga V.'
_publ_section_title
;
 (Na,Li)₃(Cl,OH)[Cu₃OAl(PO₄)₃]: a first salt-inclusion
 aluminophosphate oxocuprate with a new type of crystal structure
;
_journal_coeditor_code           JE5049
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              24
_journal_page_last               31
_journal_paper_doi               10.1107/S2052520622011696
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'Al8 Cl7 Cu24 Li4.19 Na19.81 O105 P24'
_chemical_formula_weight         4896.74
_chemical_name_common            'aluminophosphate oxocuprate'
_chemical_name_systematic        'sodium alumonophosphate oxocuprate chloride'
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                90
_cell_angle_beta                 90.361(2)
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   13.3428(4)
_cell_length_b                   18.9320(5)
_cell_length_c                   8.9404(2)
_cell_measurement_reflns_used    6699
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      37.154
_cell_measurement_theta_min      1.869
_cell_volume                     2258.35(10)
_computing_cell_refinement       'CrysAlisPro 1.171.40.67a (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.67a (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.67a (Rigaku OD, 2019)'
_computing_molecular_graphics    'Diamond (Brandenburg, 2006)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2015b)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015a)'
_diffrn_ambient_temperature      423(2)
_diffrn_detector_area_resol_mean 5.2283
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Xcalibur, AtlasS2, Gemini'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0206
_diffrn_reflns_av_unetI/netI     0.0194
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            7934
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.489
_diffrn_reflns_theta_min         1.867
_diffrn_source                   'fine-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    6.485
_exptl_absorpt_correction_T_max  1.295
_exptl_absorpt_correction_T_min  0.778
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.67a (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            light-green
_exptl_crystal_density_diffrn    3.601
_exptl_crystal_description       prism
_exptl_crystal_F_000             2349
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.045
_exptl_crystal_size_min          0.040
_exptl_transmission_factor_max   1.000
_exptl_transmission_factor_min   0.780
_refine_diff_density_max         1.698
_refine_diff_density_min         -1.739
_refine_diff_density_rms         0.191
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.165
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     247
_refine_ls_number_reflns         2646
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.165
_refine_ls_R_factor_all          0.0405
_refine_ls_R_factor_gt           0.0390
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0500P)²+30.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1089
_refine_ls_wR_factor_ref         0.1097
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2542
_reflns_number_total             2646
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            je5049sup1.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'Direct' was changed
to 'direct' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_atom_sites_solution_secondary' value 'Diffmap' was
changed to 'difmap'.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               2109099
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.563
_shelx_estimated_absorpt_t_max   0.781
_exptl_absorpt_special_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.250000 0.250000 0.500000 0.0109(2) Uani 1 2 d S . P . .
Cu2 Cu 0.12705(5) 0.41671(3) 0.31049(7) 0.01122(16) Uani 1 1 d . . . . .
Cu3 Cu 0.000000 0.24835(5) 0.500000 0.0138(2) Uani 1 2 d S T P . .
Cu4 Cu 0.62554(8) 0.74519(3) 0.82896(7) 0.02009(19) Uani 1 1 d . . . . .
P1 P 0.12573(12) 0.26303(7) 0.19526(14) 0.0112(3) Uani 1 1 d . . . . .
P2 P 0.11905(10) 0.61919(6) 0.66727(13) 0.0068(2) Uani 1 1 d . . . . .
P3 P 0.63242(10) 0.61716(7) 0.65454(13) 0.0080(3) Uani 1 1 d . . . . .
Al1 Al 0.24664(16) 0.500000 0.5261(2) 0.0073(4) Uani 1 2 d S T P . .
Al2 Al 0.000000 0.500000 0.500000 0.0060(6) Uani 1 4 d S T P . .
Al3 Al 0.500000 0.500000 0.500000 0.0086(6) Uani 1 4 d S T P . .
Na1 Na 0.000000 0.60798(18) 1.000000 0.0116(6) Uani 1 2 d S T P . .
Na2 Na 0.74974(18) 0.61404(16) 1.0123(3) 0.0231(6) Uani 1 1 d . . . . .
Na3 Na 0.6188(3) 0.6185(2) 0.3120(4) 0.0129(12) Uani 0.556(10) 1 d . . P . .
Li1 Li 0.6222(17) 0.5757(14) 0.300(2) 0.0129(12) Uani 0.444(10) 1 d . . P . .
Na4 Na 0.504(2) 0.6190(6) 1.0348(16) 0.064(6) Uani 0.420(15) 1 d . . P . .
Li2 Li 0.504(2) 0.6190(6) 1.0348(16) 0.064(6) Uani 0.080(15) 1 d . . P . .
Cl2 Cl 0.6191(3) 0.5102(4) 1.0679(3) 0.0147(17) Uani 0.375(4) 1 d . . P . .
O15 O 0.5411(17) 0.500000 0.847(2) 0.0147(17) Uani 0.251(8) 2 d S T P . .
Cl1 Cl 0.13134(16) 0.500000 0.06802(19) 0.0146(4) Uani 1 2 d S T P . .
O1 O 0.3752(4) 0.500000 0.5926(5) 0.0088(9) Uani 1 2 d S T P . .
O2 O 0.1252(4) 0.500000 0.4326(5) 0.0064(9) Uani 1 2 d S T P . .
O3 O 0.2119(3) 0.5716(2) 0.6616(4) 0.0113(7) Uani 1 1 d . . . . .
O4 O 0.7272(3) 0.5722(2) 0.6287(4) 0.0114(8) Uani 1 1 d . . . . .
O5 O 0.0234(3) 0.5724(2) 0.6514(4) 0.0082(7) Uani 1 1 d . . . . .
O6 O 0.1167(3) 0.65488(18) 0.8223(4) 0.0084(7) Uani 1 1 d . . . . .
O7 O 0.6308(3) 0.6793(2) 0.5442(4) 0.0182(8) Uani 1 1 d . . . . .
O8 O 0.1191(3) 0.6728(2) 0.5402(4) 0.0156(8) Uani 1 1 d . . . . .
O9 O 0.5405(3) 0.5711(2) 0.6362(4) 0.0136(8) Uani 1 1 d . . . . .
O10 O 0.6358(3) 0.64578(18) 0.8147(4) 0.0097(7) Uani 1 1 d . . . . .
O11 O 0.2212(3) 0.2434(2) 0.2855(5) 0.0147(8) Uani 1 1 d . . . . .
O12 O 0.0305(3) 0.2412(2) 0.2816(5) 0.0185(9) Uani 1 1 d . . . . .
O13 O 0.1248(3) 0.34339(19) 0.1676(4) 0.0102(7) Uani 1 1 d . . . . .
O14 O 0.1273(5) 0.2248(2) 0.0484(5) 0.0360(12) Uani 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O11 Cu1 O11 180.0 7_556 . ?
O11 Cu1 O7 89.97(16) 7_556 5_666 ?
O11 Cu1 O7 90.03(16) . 5_666 ?
O11 Cu1 O7 90.03(16) 7_556 3_445 ?
O11 Cu1 O7 89.97(16) . 3_445 ?
O7 Cu1 O7 180.00(17) 5_666 3_445 ?
O11 Cu1 O8 87.20(14) 7_556 6_565 ?
O11 Cu1 O8 92.80(14) . 6_565 ?
O7 Cu1 O8 101.48(16) 5_666 6_565 ?
O7 Cu1 O8 78.52(16) 3_445 6_565 ?
O11 Cu1 O8 92.80(14) 7_556 4_546 ?
O11 Cu1 O8 87.20(14) . 4_546 ?
O7 Cu1 O8 78.52(16) 5_666 4_546 ?
O7 Cu1 O8 101.48(16) 3_445 4_546 ?
O8 Cu1 O8 180.0 6_565 4_546 ?
O11 Cu1 Na3 127.99(14) 7_556 3_445 ?
O11 Cu1 Na3 52.01(14) . 3_445 ?
O7 Cu1 Na3 137.72(12) 5_666 3_445 ?
O7 Cu1 Na3 42.28(12) 3_445 3_445 ?
O8 Cu1 Na3 98.60(12) 6_565 3_445 ?
O8 Cu1 Na3 81.40(12) 4_546 3_445 ?
O11 Cu1 Na3 52.01(14) 7_556 5_666 ?
O11 Cu1 Na3 127.99(14) . 5_666 ?
O7 Cu1 Na3 42.28(12) 5_666 5_666 ?
O7 Cu1 Na3 137.72(12) 3_445 5_666 ?
O8 Cu1 Na3 81.40(12) 6_565 5_666 ?
O8 Cu1 Na3 98.60(12) 4_546 5_666 ?
Na3 Cu1 Na3 180.00(9) 3_445 5_666 ?
O13 Cu2 O2 171.92(16) . . ?
O13 Cu2 O4 105.60(16) . 5_666 ?
O2 Cu2 O4 77.17(19) . 5_666 ?
O13 Cu2 O5 100.09(15) . 5_566 ?
O2 Cu2 O5 78.85(19) . 5_566 ?
O4 Cu2 O5 152.18(14) 5_666 5_566 ?
O13 Cu2 Cl1 83.43(11) . . ?
O2 Cu2 Cl1 88.69(11) . . ?
O4 Cu2 Cl1 97.51(12) 5_666 . ?
O5 Cu2 Cl1 95.82(11) 5_566 . ?
O13 Cu2 Al2 142.71(12) . . ?
O2 Cu2 Al2 37.26(16) . . ?
O4 Cu2 Al2 110.70(11) 5_666 . ?
O5 Cu2 Al2 42.68(10) 5_566 . ?
Cl1 Cu2 Al2 99.76(4) . . ?
O13 Cu2 Al1 147.31(12) . . ?
O2 Cu2 Al1 36.66(16) . . ?
O4 Cu2 Al1 41.89(11) 5_666 . ?
O5 Cu2 Al1 111.35(11) 5_566 . ?
Cl1 Cu2 Al1 101.51(5) . . ?
Al2 Cu2 Al1 68.93(4) . . ?
O13 Cu2 Na1 46.81(12) . 5_566 ?
O2 Cu2 Na1 126.23(15) . 5_566 ?
O4 Cu2 Na1 137.09(11) 5_666 5_566 ?
O5 Cu2 Na1 69.70(10) 5_566 5_566 ?
Cl1 Cu2 Na1 54.03(6) . 5_566 ?
Al2 Cu2 Na1 105.88(4) . 5_566 ?
Al1 Cu2 Na1 154.72(6) . 5_566 ?
O13 Cu2 Na2 45.66(12) . 5_666 ?
O2 Cu2 Na2 129.45(14) . 5_666 ?
O4 Cu2 Na2 77.06(11) 5_666 5_666 ?
O5 Cu2 Na2 129.91(11) 5_566 5_666 ?
Cl1 Cu2 Na2 53.00(6) . 5_666 ?
Al2 Cu2 Na2 152.76(5) . 5_666 ?
Al1 Cu2 Na2 112.69(6) . 5_666 ?
Na1 Cu2 Na2 60.27(4) 5_566 5_666 ?
O12 Cu3 O12 172.3(3) 2_556 . ?
O12 Cu3 O8 92.15(16) 2_556 6_565 ?
O12 Cu3 O8 93.07(15) . 6_565 ?
O12 Cu3 O8 93.07(15) 2_556 5_566 ?
O12 Cu3 O8 92.15(16) . 5_566 ?
O8 Cu3 O8 94.9(2) 6_565 5_566 ?
O12 Cu3 O7 88.25(16) 2_556 4_546 ?
O12 Cu3 O7 87.19(16) . 4_546 ?
O8 Cu3 O7 173.64(16) 6_565 4_546 ?
O8 Cu3 O7 78.74(16) 5_566 4_546 ?
O12 Cu3 O7 87.19(16) 2_556 3_445 ?
O12 Cu3 O7 88.24(16) . 3_445 ?
O8 Cu3 O7 78.74(16) 6_565 3_445 ?
O8 Cu3 O7 173.64(16) 5_566 3_445 ?
O7 Cu3 O7 107.6(2) 4_546 3_445 ?
O12 Cu3 Na3 122.37(14) 2_556 3_445 ?
O12 Cu3 Na3 50.70(14) . 3_445 ?
O8 Cu3 Na3 103.50(12) 6_565 3_445 ?
O8 Cu3 Na3 138.63(12) 5_566 3_445 ?
O7 Cu3 Na3 81.57(13) 4_546 3_445 ?
O7 Cu3 Na3 44.56(12) 3_445 3_445 ?
O12 Cu3 Na3 50.70(14) 2_556 4_546 ?
O12 Cu3 Na3 122.37(14) . 4_546 ?
O8 Cu3 Na3 138.63(12) 6_565 4_546 ?
O8 Cu3 Na3 103.50(12) 5_566 4_546 ?
O7 Cu3 Na3 44.56(12) 4_546 4_546 ?
O7 Cu3 Na3 81.57(13) 3_445 4_546 ?
Na3 Cu3 Na3 86.65(13) 3_445 4_546 ?
O10 Cu4 O6 174.30(14) . 8_565 ?
O10 Cu4 O14 82.72(17) . 3_556 ?
O6 Cu4 O14 102.96(17) 8_565 3_556 ?
O10 Cu4 O12 90.24(16) . 4_556 ?
O6 Cu4 O12 87.89(16) 8_565 4_556 ?
O14 Cu4 O12 114.9(2) 3_556 4_556 ?
O10 Cu4 O11 89.92(15) . 5_666 ?
O6 Cu4 O11 86.99(15) 8_565 5_666 ?
O14 Cu4 O11 116.7(2) 3_556 5_666 ?
O12 Cu4 O11 128.04(14) 4_556 5_666 ?
O10 Cu4 Na4 47.3(4) . 2_657 ?
O6 Cu4 Na4 136.4(4) 8_565 2_657 ?
O14 Cu4 Na4 59.0(3) 3_556 2_657 ?
O12 Cu4 Na4 69.4(4) 4_556 2_657 ?
O11 Cu4 Na4 136.4(4) 5_666 2_657 ?
O10 Cu4 Na2 43.18(12) . . ?
O6 Cu4 Na2 140.67(13) 8_565 . ?
O14 Cu4 Na2 51.90(16) 3_556 . ?
O12 Cu4 Na2 128.34(13) 4_556 . ?
O11 Cu4 Na2 81.45(11) 5_666 . ?
Na4 Cu4 Na2 62.3(4) 2_657 . ?
O10 Cu4 Na4 51.5(3) . . ?
O6 Cu4 Na4 133.1(3) 8_565 . ?
O14 Cu4 Na4 48.8(3) 3_556 . ?
O12 Cu4 Na4 77.2(4) 4_556 . ?
O11 Cu4 Na4 136.7(4) 5_666 . ?
Na4 Cu4 Na4 10.2(5) 2_657 . ?
Na2 Cu4 Na4 57.5(4) . . ?
O10 Cu4 Na2 139.73(13) . 7_667 ?
O6 Cu4 Na2 43.15(12) 8_565 7_667 ?
O14 Cu4 Na2 75.09(17) 3_556 7_667 ?
O12 Cu4 Na2 129.50(12) 4_556 7_667 ?
O11 Cu4 Na2 71.47(12) 5_666 7_667 ?
Na4 Cu4 Na2 133.1(3) 2_657 7_667 ?
Na2 Cu4 Na2 97.69(7) . 7_667 ?
Na4 Cu4 Na2 123.1(2) . 7_667 ?
O10 Cu4 Na1 146.39(12) . 7_567 ?
O6 Cu4 Na1 38.04(11) 8_565 7_567 ?
O14 Cu4 Na1 74.62(15) 3_556 7_567 ?
O12 Cu4 Na1 77.57(11) 4_556 7_567 ?
O11 Cu4 Na1 122.30(11) 5_666 7_567 ?
Na4 Cu4 Na1 99.2(4) 2_657 7_567 ?
Na2 Cu4 Na1 125.94(5) . 7_567 ?
Na4 Cu4 Na1 95.1(3) . 7_567 ?
Na2 Cu4 Na1 56.71(5) 7_667 7_567 ?
O14 P1 O13 109.7(2) . . ?
O14 P1 O12 108.9(3) . . ?
O13 P1 O12 109.7(2) . . ?
O14 P1 O11 108.9(3) . . ?
O13 P1 O11 109.0(2) . . ?
O12 P1 O11 110.6(2) . . ?
O14 P1 Na3 82.0(2) . 3_445 ?
O13 P1 Na3 168.12(16) . 3_445 ?
O12 P1 Na3 62.95(19) . 3_445 ?
O11 P1 Na3 67.54(18) . 3_445 ?
O14 P1 Na2 81.0(2) . 5_666 ?
O13 P1 Na2 40.85(14) . 5_666 ?
O12 P1 Na2 149.00(18) . 5_666 ?
O11 P1 Na2 92.59(17) . 5_666 ?
Na3 P1 Na2 147.83(10) 3_445 5_666 ?
O14 P1 Na1 84.7(2) . 5_566 ?
O13 P1 Na1 38.10(15) . 5_566 ?
O12 P1 Na1 92.48(17) . 5_566 ?
O11 P1 Na1 146.43(17) . 5_566 ?
Na3 P1 Na1 145.98(10) 3_445 5_566 ?
Na2 P1 Na1 58.45(5) 5_666 5_566 ?
O8 P2 O3 111.3(2) . . ?
O8 P2 O6 112.2(2) . . ?
O3 P2 O6 107.9(2) . . ?
O8 P2 O5 108.3(2) . . ?
O3 P2 O5 108.9(2) . . ?
O6 P2 O5 108.0(2) . . ?
O8 P2 Na2 130.91(17) . 2_657 ?
O3 P2 Na2 65.98(16) . 2_657 ?
O6 P2 Na2 42.06(15) . 2_657 ?
O5 P2 Na2 118.99(15) . 2_657 ?
O8 P2 Na1 134.34(18) . . ?
O3 P2 Na1 112.06(16) . . ?
O6 P2 Na1 39.30(14) . . ?
O5 P2 Na1 69.90(14) . . ?
Na2 P2 Na1 59.51(5) 2_657 . ?
O9 P3 O10 108.9(2) . . ?
O9 P3 O7 111.3(3) . . ?
O10 P3 O7 109.3(2) . . ?
O9 P3 O4 109.3(2) . . ?
O10 P3 O4 108.4(2) . . ?
O7 P3 O4 109.6(2) . . ?
O9 P3 Na3 81.60(18) . . ?
O10 P3 Na3 158.74(17) . . ?
O7 P3 Na3 49.57(17) . . ?
O4 P3 Na3 84.16(17) . . ?
O9 P3 Na4 69.4(4) . 2_657 ?
O10 P3 Na4 39.7(4) . 2_657 ?
O7 P3 Na4 121.5(3) . 2_657 ?
O4 P3 Na4 125.8(4) . 2_657 ?
Na3 P3 Na4 143.4(4) . 2_657 ?
O9 P3 Na3 37.58(17) . 2_656 ?
O10 P3 Na3 86.42(17) . 2_656 ?
O7 P3 Na3 92.4(2) . 2_656 ?
O4 P3 Na3 146.60(17) . 2_656 ?
Na3 P3 Na3 92.07(10) . 2_656 ?
Na4 P3 Na3 51.3(4) 2_657 2_656 ?
O1 Al1 O2 171.8(3) . . ?
O1 Al1 O3 91.46(18) . 6_565 ?
O2 Al1 O3 94.22(17) . 6_565 ?
O1 Al1 O3 91.46(18) . . ?
O2 Al1 O3 94.22(17) . . ?
O3 Al1 O3 92.4(3) 6_565 . ?
O1 Al1 O4 93.36(18) . 5_666 ?
O2 Al1 O4 80.74(17) . 5_666 ?
O3 Al1 O4 89.88(17) 6_565 5_666 ?
O3 Al1 O4 174.6(2) . 5_666 ?
O1 Al1 O4 93.35(18) . 2_656 ?
O2 Al1 O4 80.74(17) . 2_656 ?
O3 Al1 O4 174.6(2) 6_565 2_656 ?
O3 Al1 O4 89.88(17) . 2_656 ?
O4 Al1 O4 87.5(2) 5_666 2_656 ?
O1 Al1 Li1 38.1(5) . 2_656 ?
O2 Al1 Li1 145.6(5) . 2_656 ?
O3 Al1 Li1 99.9(5) 6_565 2_656 ?
O3 Al1 Li1 54.3(5) . 2_656 ?
O4 Al1 Li1 130.1(5) 5_666 2_656 ?
O4 Al1 Li1 85.4(5) 2_656 2_656 ?
O1 Al1 Li1 38.1(5) . 5_666 ?
O2 Al1 Li1 145.6(5) . 5_666 ?
O3 Al1 Li1 54.3(5) 6_565 5_666 ?
O3 Al1 Li1 99.9(5) . 5_666 ?
O4 Al1 Li1 85.4(5) 5_666 5_666 ?
O4 Al1 Li1 130.1(5) 2_656 5_666 ?
Li1 Al1 Li1 63.1(11) 2_656 5_666 ?
O1 Al1 Cu2 136.15(12) . . ?
O2 Al1 Cu2 39.04(8) . . ?
O3 Al1 Cu2 84.33(13) 6_565 . ?
O3 Al1 Cu2 132.24(15) . . ?
O4 Al1 Cu2 43.18(12) 5_666 . ?
O4 Al1 Cu2 90.55(14) 2_656 . ?
Li1 Al1 Cu2 172.5(4) 2_656 . ?
Li1 Al1 Cu2 115.6(5) 5_666 . ?
O1 Al1 Cu2 136.15(12) . 6_565 ?
O2 Al1 Cu2 39.04(8) . 6_565 ?
O3 Al1 Cu2 132.24(15) 6_565 6_565 ?
O3 Al1 Cu2 84.33(13) . 6_565 ?
O4 Al1 Cu2 90.55(14) 5_666 6_565 ?
O4 Al1 Cu2 43.18(12) 2_656 6_565 ?
Li1 Al1 Cu2 115.6(5) 2_656 6_565 ?
Li1 Al1 Cu2 172.5(4) 5_666 6_565 ?
Cu2 Al1 Cu2 64.60(5) . 6_565 ?
O1 Al1 Na3 47.70(9) . 2_656 ?
O2 Al1 Na3 134.50(9) . 2_656 ?
O3 Al1 Na3 110.66(17) 6_565 2_656 ?
O3 Al1 Na3 49.06(14) . 2_656 ?
O4 Al1 Na3 134.23(15) 5_666 2_656 ?
O4 Al1 Na3 74.45(14) 2_656 2_656 ?
Li1 Al1 Na3 12.9(5) 2_656 2_656 ?
Li1 Al1 Na3 75.9(6) 5_666 2_656 ?
Cu2 Al1 Na3 164.98(10) . 2_656 ?
Cu2 Al1 Na3 102.68(8) 6_565 2_656 ?
O1 Al1 Na3 47.70(9) . 5_666 ?
O2 Al1 Na3 134.50(9) . 5_666 ?
O3 Al1 Na3 49.06(14) 6_565 5_666 ?
O3 Al1 Na3 110.66(16) . 5_666 ?
O4 Al1 Na3 74.45(14) 5_666 5_666 ?
O4 Al1 Na3 134.23(15) 2_656 5_666 ?
Li1 Al1 Na3 75.9(6) 2_656 5_666 ?
Li1 Al1 Na3 12.9(5) 5_666 5_666 ?
Cu2 Al1 Na3 102.68(8) . 5_666 ?
Cu2 Al1 Na3 164.98(10) 6_565 5_666 ?
Na3 Al1 Na3 88.61(16) 2_656 5_666 ?
O2 Al2 O2 180.0 . 5_566 ?
O2 Al2 O5 95.08(15) . . ?
O2 Al2 O5 84.92(15) 5_566 . ?
O2 Al2 O5 84.92(15) . 5_566 ?
O2 Al2 O5 95.08(15) 5_566 5_566 ?
O5 Al2 O5 180.0 . 5_566 ?
O2 Al2 O5 95.08(15) . 6_565 ?
O2 Al2 O5 84.92(15) 5_566 6_565 ?
O5 Al2 O5 89.3(2) . 6_565 ?
O5 Al2 O5 90.7(2) 5_566 6_565 ?
O2 Al2 O5 84.92(15) . 2_556 ?
O2 Al2 O5 95.08(15) 5_566 2_556 ?
O5 Al2 O5 90.7(2) . 2_556 ?
O5 Al2 O5 89.3(2) 5_566 2_556 ?
O5 Al2 O5 180.0 6_565 2_556 ?
O2 Al2 Cu2 40.73(8) . . ?
O2 Al2 Cu2 139.27(8) 5_566 . ?
O5 Al2 Cu2 134.60(10) . . ?
O5 Al2 Cu2 45.40(10) 5_566 . ?
O5 Al2 Cu2 86.04(11) 6_565 . ?
O5 Al2 Cu2 93.96(11) 2_556 . ?
O2 Al2 Cu2 139.27(8) . 2_556 ?
O2 Al2 Cu2 40.73(8) 5_566 2_556 ?
O5 Al2 Cu2 93.96(11) . 2_556 ?
O5 Al2 Cu2 86.04(11) 5_566 2_556 ?
O5 Al2 Cu2 45.40(10) 6_565 2_556 ?
O5 Al2 Cu2 134.60(10) 2_556 2_556 ?
Cu2 Al2 Cu2 113.48(3) . 2_556 ?
O2 Al2 Cu2 139.27(8) . 5_566 ?
O2 Al2 Cu2 40.73(8) 5_566 5_566 ?
O5 Al2 Cu2 45.40(10) . 5_566 ?
O5 Al2 Cu2 134.60(10) 5_566 5_566 ?
O5 Al2 Cu2 93.96(11) 6_565 5_566 ?
O5 Al2 Cu2 86.04(11) 2_556 5_566 ?
Cu2 Al2 Cu2 180.00(2) . 5_566 ?
Cu2 Al2 Cu2 66.52(3) 2_556 5_566 ?
O2 Al2 Cu2 40.73(8) . 6_565 ?
O2 Al2 Cu2 139.27(8) 5_566 6_565 ?
O5 Al2 Cu2 86.04(11) . 6_565 ?
O5 Al2 Cu2 93.96(11) 5_566 6_565 ?
O5 Al2 Cu2 134.60(10) 6_565 6_565 ?
O5 Al2 Cu2 45.40(10) 2_556 6_565 ?
Cu2 Al2 Cu2 66.52(3) . 6_565 ?
Cu2 Al2 Cu2 180.00(2) 2_556 6_565 ?
Cu2 Al2 Cu2 113.48(3) 5_566 6_565 ?
O1 Al3 O1 180.0 5_666 . ?
O1 Al3 O9 88.09(16) 5_666 5_666 ?
O1 Al3 O9 91.91(16) . 5_666 ?
O1 Al3 O9 91.91(16) 5_666 6_565 ?
O1 Al3 O9 88.09(16) . 6_565 ?
O9 Al3 O9 89.3(3) 5_666 6_565 ?
O1 Al3 O9 88.09(16) 5_666 2_656 ?
O1 Al3 O9 91.91(16) . 2_656 ?
O9 Al3 O9 90.7(3) 5_666 2_656 ?
O9 Al3 O9 180.0 6_565 2_656 ?
O1 Al3 O9 91.91(16) 5_666 . ?
O1 Al3 O9 88.09(16) . . ?
O9 Al3 O9 180.0 5_666 . ?
O9 Al3 O9 90.7(3) 6_565 . ?
O9 Al3 O9 89.3(3) 2_656 . ?
O1 Al3 Li1 36.5(5) 5_666 6_565 ?
O1 Al3 Li1 143.5(5) . 6_565 ?
O9 Al3 Li1 52.7(5) 5_666 6_565 ?
O9 Al3 Li1 83.2(5) 6_565 6_565 ?
O9 Al3 Li1 96.8(5) 2_656 6_565 ?
O9 Al3 Li1 127.3(5) . 6_565 ?
O1 Al3 Li1 143.5(5) 5_666 2_656 ?
O1 Al3 Li1 36.5(5) . 2_656 ?
O9 Al3 Li1 127.3(5) 5_666 2_656 ?
O9 Al3 Li1 96.8(5) 6_565 2_656 ?
O9 Al3 Li1 83.2(5) 2_656 2_656 ?
O9 Al3 Li1 52.7(5) . 2_656 ?
Li1 Al3 Li1 180.0 6_565 2_656 ?
O1 Al3 Li1 143.5(5) 5_666 5_666 ?
O1 Al3 Li1 36.5(5) . 5_666 ?
O9 Al3 Li1 83.2(5) 5_666 5_666 ?
O9 Al3 Li1 52.7(5) 6_565 5_666 ?
O9 Al3 Li1 127.3(5) 2_656 5_666 ?
O9 Al3 Li1 96.8(5) . 5_666 ?
Li1 Al3 Li1 118.8(10) 6_565 5_666 ?
Li1 Al3 Li1 61.2(10) 2_656 5_666 ?
O1 Al3 Li1 36.5(5) 5_666 . ?
O1 Al3 Li1 143.5(5) . . ?
O9 Al3 Li1 96.8(5) 5_666 . ?
O9 Al3 Li1 127.3(5) 6_565 . ?
O9 Al3 Li1 52.7(5) 2_656 . ?
O9 Al3 Li1 83.2(5) . . ?
Li1 Al3 Li1 61.2(10) 6_565 . ?
Li1 Al3 Li1 118.8(10) 2_656 . ?
Li1 Al3 Li1 180.0 5_666 . ?
O1 Al3 Na3 47.57(9) 5_666 . ?
O1 Al3 Na3 132.43(9) . . ?
O9 Al3 Na3 107.38(14) 5_666 . ?
O9 Al3 Na3 133.70(14) 6_565 . ?
O9 Al3 Na3 46.30(14) 2_656 . ?
O9 Al3 Na3 72.62(14) . . ?
Li1 Al3 Na3 74.7(5) 6_565 . ?
Li1 Al3 Na3 105.3(5) 2_656 . ?
Li1 Al3 Na3 166.5(5) 5_666 . ?
Li1 Al3 Na3 13.5(5) . . ?
O1 Al3 Na3 132.43(9) 5_666 2_656 ?
O1 Al3 Na3 47.57(9) . 2_656 ?
O9 Al3 Na3 133.70(14) 5_666 2_656 ?
O9 Al3 Na3 107.38(14) 6_565 2_656 ?
O9 Al3 Na3 72.62(14) 2_656 2_656 ?
O9 Al3 Na3 46.30(14) . 2_656 ?
Li1 Al3 Na3 166.5(5) 6_565 2_656 ?
Li1 Al3 Na3 13.5(5) 2_656 2_656 ?
Li1 Al3 Na3 74.7(5) 5_666 2_656 ?
Li1 Al3 Na3 105.3(5) . 2_656 ?
Na3 Al3 Na3 91.86(14) . 2_656 ?
O6 Na1 O6 136.6(2) . 2_557 ?
O6 Na1 O13 79.75(12) . 6_566 ?
O6 Na1 O13 84.04(13) 2_557 6_566 ?
O6 Na1 O13 84.04(13) . 5_566 ?
O6 Na1 O13 79.75(12) 2_557 5_566 ?
O13 Na1 O13 135.2(2) 6_566 5_566 ?
O6 Na1 Cl1 122.81(10) . 5_566 ?
O6 Na1 Cl1 90.35(10) 2_557 5_566 ?
O13 Na1 Cl1 148.63(13) 6_566 5_566 ?
O13 Na1 Cl1 73.21(10) 5_566 5_566 ?
O6 Na1 Cl1 90.35(10) . 1_556 ?
O6 Na1 Cl1 122.81(10) 2_557 1_556 ?
O13 Na1 Cl1 73.21(10) 6_566 1_556 ?
O13 Na1 Cl1 148.63(13) 5_566 1_556 ?
Cl1 Na1 Cl1 84.32(11) 5_566 1_556 ?
O6 Na1 Cu2 80.01(9) . 5_566 ?
O6 Na1 Cu2 106.19(9) 2_557 5_566 ?
O13 Na1 Cu2 158.56(12) 6_566 5_566 ?
O13 Na1 Cu2 34.70(8) 5_566 5_566 ?
Cl1 Na1 Cu2 51.89(4) 5_566 5_566 ?
Cl1 Na1 Cu2 113.93(9) 1_556 5_566 ?
O6 Na1 Cu2 106.19(9) . 6_566 ?
O6 Na1 Cu2 80.01(9) 2_557 6_566 ?
O13 Na1 Cu2 34.70(8) 6_566 6_566 ?
O13 Na1 Cu2 158.56(12) 5_566 6_566 ?
Cl1 Na1 Cu2 113.93(9) 5_566 6_566 ?
Cl1 Na1 Cu2 51.89(4) 1_556 6_566 ?
Cu2 Na1 Cu2 163.60(12) 5_566 6_566 ?
O6 Na1 Na2 46.66(10) . 2_657 ?
O6 Na1 Na2 131.38(12) 2_557 2_657 ?
O13 Na1 Na2 47.37(10) 6_566 2_657 ?
O13 Na1 Na2 130.63(11) 5_566 2_657 ?
Cl1 Na1 Na2 130.65(12) 5_566 2_657 ?
Cl1 Na1 Na2 53.09(6) 1_556 2_657 ?
Cu2 Na1 Na2 119.23(5) 5_566 2_657 ?
Cu2 Na1 Na2 61.41(5) 6_566 2_657 ?
O6 Na1 Na2 131.38(12) . 1_455 ?
O6 Na1 Na2 46.66(10) 2_557 1_455 ?
O13 Na1 Na2 130.63(11) 6_566 1_455 ?
O13 Na1 Na2 47.37(10) 5_566 1_455 ?
Cl1 Na1 Na2 53.09(6) 5_566 1_455 ?
Cl1 Na1 Na2 130.65(12) 1_556 1_455 ?
Cu2 Na1 Na2 61.41(5) 5_566 1_455 ?
Cu2 Na1 Na2 119.23(5) 6_566 1_455 ?
Na2 Na1 Na2 176.07(16) 2_657 1_455 ?
O6 Na1 P2 150.14(14) . 2_557 ?
O6 Na1 P2 24.01(8) 2_557 2_557 ?
O13 Na1 P2 75.91(9) 6_566 2_557 ?
O13 Na1 P2 101.28(9) 5_566 2_557 ?
Cl1 Na1 P2 86.52(6) 5_566 2_557 ?
Cl1 Na1 P2 98.83(6) 1_556 2_557 ?
Cu2 Na1 P2 120.65(3) 5_566 2_557 ?
Cu2 Na1 P2 60.53(2) 6_566 2_557 ?
Na2 Na1 P2 120.05(5) 2_657 2_557 ?
Na2 Na1 P2 59.67(5) 1_455 2_557 ?
O6 Na1 P2 24.00(8) . . ?
O6 Na1 P2 150.14(14) 2_557 . ?
O13 Na1 P2 101.28(9) 6_566 . ?
O13 Na1 P2 75.91(9) 5_566 . ?
Cl1 Na1 P2 98.83(6) 5_566 . ?
Cl1 Na1 P2 86.52(6) 1_556 . ?
Cu2 Na1 P2 60.53(2) 5_566 . ?
Cu2 Na1 P2 120.65(3) 6_566 . ?
Na2 Na1 P2 59.67(5) 2_657 . ?
Na2 Na1 P2 120.05(5) 1_455 . ?
P2 Na1 P2 172.82(12) 2_557 . ?
O10 Na2 O6 145.63(18) . 2_657 ?
O10 Na2 O13 82.37(15) . 5_666 ?
O6 Na2 O13 78.17(13) 2_657 5_666 ?
O10 Na2 Cl2 84.84(14) . . ?
O6 Na2 Cl2 126.58(15) 2_657 . ?
O13 Na2 Cl2 143.84(17) 5_666 . ?
O10 Na2 O14 60.57(15) . 3_556 ?
O6 Na2 O14 97.06(18) 2_657 3_556 ?
O13 Na2 O14 103.87(18) 5_666 3_556 ?
Cl2 Na2 O14 98.9(2) . 3_556 ?
O10 Na2 Cl1 111.38(13) . 5_666 ?
O6 Na2 Cl1 89.25(12) 2_657 5_666 ?
O13 Na2 Cl1 72.17(11) 5_666 5_666 ?
Cl2 Na2 Cl1 81.43(16) . 5_666 ?
O14 Na2 Cl1 171.77(15) 3_556 5_666 ?
O10 Na2 Cl2 87.23(14) . 6_565 ?
O6 Na2 Cl2 125.31(15) 2_657 6_565 ?
O13 Na2 Cl2 140.31(16) 5_666 6_565 ?
Cl2 Na2 Cl2 5.1(2) . 6_565 ?
O14 Na2 Cl2 103.93(19) 3_556 6_565 ?
Cl1 Na2 Cl2 76.38(14) 5_666 6_565 ?
O10 Na2 Li1 108.3(4) . 1_556 ?
O6 Na2 Li1 88.5(4) 2_657 1_556 ?
O13 Na2 Li1 166.6(5) 5_666 1_556 ?
Cl2 Na2 Li1 47.9(5) . 1_556 ?
O14 Na2 Li1 75.6(5) 3_556 1_556 ?
Cl1 Na2 Li1 110.0(5) 5_666 1_556 ?
Cl2 Na2 Li1 50.7(5) 6_565 1_556 ?
O10 Na2 Na3 105.21(14) . 1_556 ?
O6 Na2 Na3 83.38(13) 2_657 1_556 ?
O13 Na2 Na3 155.79(16) 5_666 1_556 ?
Cl2 Na2 Na3 60.37(13) . 1_556 ?
O14 Na2 Na3 62.82(14) 3_556 1_556 ?
Cl1 Na2 Na3 123.48(12) 5_666 1_556 ?
Cl2 Na2 Na3 63.79(12) 6_565 1_556 ?
Li1 Na2 Na3 14.7(5) 1_556 1_556 ?
O10 Na2 Na4 53.9(3) . . ?
O6 Na2 Na4 132.9(3) 2_657 . ?
O13 Na2 Na4 135.4(3) 5_666 . ?
Cl2 Na2 Na4 50.1(2) . . ?
O14 Na2 Na4 50.3(2) 3_556 . ?
Cl1 Na2 Na4 127.6(2) 5_666 . ?
Cl2 Na2 Na4 55.0(2) 6_565 . ?
Li1 Na2 Na4 54.4(5) 1_556 . ?
Na3 Na2 Na4 53.1(3) 1_556 . ?
O10 Na2 Na1 127.76(13) . 1_655 ?
O6 Na2 Na1 45.86(10) 2_657 1_655 ?
O13 Na2 Na1 46.14(10) 5_666 1_655 ?
Cl2 Na2 Na1 129.27(17) . 1_655 ?
O14 Na2 Na1 129.84(18) 3_556 1_655 ?
Cl1 Na2 Na1 52.58(8) 5_666 1_655 ?
Cl2 Na2 Na1 124.43(16) 6_565 1_655 ?
Li1 Na2 Na1 124.0(4) 1_556 1_655 ?
Na3 Na2 Na1 125.28(11) 1_556 1_655 ?
Na4 Na2 Na1 178.3(3) . 1_655 ?
Li1 Na3 O9 72.4(16) . 2_656 ?
Li1 Na3 O7 126.0(16) . . ?
O9 Na3 O7 93.9(2) 2_656 . ?
Li1 Na3 O1 28.2(15) . 5_666 ?
O9 Na3 O1 66.54(19) 2_656 5_666 ?
O7 Na3 O1 98.0(2) . 5_666 ?
Li1 Na3 O3 66.4(17) . 2_656 ?
O9 Na3 O3 132.7(2) 2_656 2_656 ?
O7 Na3 O3 92.0(2) . 2_656 ?
O1 Na3 O3 66.20(19) 5_666 2_656 ?
Li1 Na3 O12 152.9(17) . 3 ?
O9 Na3 O12 87.29(19) 2_656 3 ?
O7 Na3 O12 71.88(18) . 3 ?
O1 Na3 O12 151.6(2) 5_666 3 ?
O3 Na3 O12 138.6(2) 2_656 3 ?
Li1 Na3 O11 144.6(16) . 3 ?
O9 Na3 O11 142.8(2) 2_656 3 ?
O7 Na3 O11 68.13(17) . 3 ?
O1 Na3 O11 145.2(2) 5_666 3 ?
O3 Na3 O11 81.99(17) 2_656 3 ?
O12 Na3 O11 56.63(14) 3 3 ?
Li1 Na3 Na4 85.5(17) . 1_554 ?
O9 Na3 Na4 72.5(5) 2_656 1_554 ?
O7 Na3 Na4 140.9(4) . 1_554 ?
O1 Na3 Na4 108.8(3) 5_666 1_554 ?
O3 Na3 Na4 124.5(5) 2_656 1_554 ?
O12 Na3 Na4 71.0(3) 3 1_554 ?
O11 Na3 Na4 100.6(4) 3 1_554 ?
Li1 Na3 P1 151.3(15) . 3 ?
O9 Na3 P1 117.15(18) 2_656 3 ?
O7 Na3 P1 81.78(15) . 3 ?
O1 Na3 P1 176.3(2) 5_666 3 ?
O3 Na3 P1 110.11(17) 2_656 3 ?
O12 Na3 P1 31.74(11) 3 3 ?
O11 Na3 P1 31.48(10) 3 3 ?
Na4 Na3 P1 73.2(3) 1_554 3 ?
Li1 Na3 Cl2 39.5(15) . 1_554 ?
O9 Na3 Cl2 83.54(18) 2_656 1_554 ?
O7 Na3 Cl2 165.3(2) . 1_554 ?
O1 Na3 Cl2 67.62(19) 5_666 1_554 ?
O3 Na3 Cl2 79.38(16) 2_656 1_554 ?
O12 Na3 Cl2 122.3(2) 3 1_554 ?
O11 Na3 Cl2 121.65(19) 3 1_554 ?
Na4 Na3 Cl2 51.9(3) 1_554 1_554 ?
P1 Na3 Cl2 112.31(17) 3 1_554 ?
Li1 Na3 P3 96.7(15) . . ?
O9 Na3 P3 81.27(15) 2_656 . ?
O7 Na3 P3 29.43(11) . . ?
O1 Na3 P3 68.63(15) 5_666 . ?
O3 Na3 P3 81.44(15) 2_656 . ?
O12 Na3 P3 97.75(16) 3 . ?
O11 Na3 P3 93.85(15) 3 . ?
Na4 Na3 P3 151.7(5) 1_554 . ?
P1 Na3 P3 111.20(14) 3 . ?
Cl2 Na3 P3 136.19(19) 1_554 . ?
Li1 Na3 Na2 80.6(15) . 1_554 ?
O9 Na3 Na2 130.6(2) 2_656 1_554 ?
O7 Na3 Na2 135.06(19) . 1_554 ?
O1 Na3 Na2 104.78(18) 5_666 1_554 ?
O3 Na3 Na2 64.03(13) 2_656 1_554 ?
O12 Na3 Na2 100.59(16) 3 1_554 ?
O11 Na3 Na2 71.13(13) 3 1_554 ?
Na4 Na3 Na2 64.7(5) 1_554 1_554 ?
P1 Na3 Na2 73.07(10) 3 1_554 ?
Cl2 Na3 Na2 50.97(13) 1_554 1_554 ?
P3 Na3 Na2 143.56(15) . 1_554 ?
Na3 Li1 O1 139(2) . 5_666 ?
Na3 Li1 O3 94.0(18) . 2_656 ?
O1 Li1 O3 82.5(9) 5_666 2_656 ?
Na3 Li1 O9 87.3(17) . 2_656 ?
O1 Li1 O9 81.0(9) 5_666 2_656 ?
O3 Li1 O9 156.2(11) 2_656 2_656 ?
Na3 Li1 Cl2 128.1(19) . 1_554 ?
O1 Li1 Cl2 92.9(11) 5_666 1_554 ?
O3 Li1 Cl2 97.2(8) 2_656 1_554 ?
O9 Li1 Cl2 100.7(9) 2_656 1_554 ?
Na3 Li1 Cl2 135.3(19) . 6_564 ?
O1 Li1 Cl2 85.7(10) 5_666 6_564 ?
O3 Li1 Cl2 96.3(8) 2_656 6_564 ?
O9 Li1 Cl2 99.5(9) 2_656 6_564 ?
Cl2 Li1 Cl2 7.2(3) 1_554 6_564 ?
Na3 Li1 Al1 119(2) . 5_666 ?
O1 Li1 Al1 40.5(5) 5_666 5_666 ?
O3 Li1 Al1 42.9(4) 2_656 5_666 ?
O9 Li1 Al1 116.8(9) 2_656 5_666 ?
Cl2 Li1 Al1 103.1(9) 1_554 5_666 ?
Cl2 Li1 Al1 97.5(8) 6_564 5_666 ?
Na3 Li1 Al3 112.9(18) . . ?
O1 Li1 Al3 40.0(5) 5_666 . ?
O3 Li1 Al3 117.4(9) 2_656 . ?
O9 Li1 Al3 42.0(4) 2_656 . ?
Cl2 Li1 Al3 106.1(9) 1_554 . ?
Cl2 Li1 Al3 100.3(8) 6_564 . ?
Al1 Li1 Al3 75.2(6) 5_666 . ?
Na3 Li1 Li1 172.0(15) . 6_565 ?
O1 Li1 Li1 33.8(8) 5_666 6_565 ?
O3 Li1 Li1 88.0(7) 2_656 6_565 ?
O9 Li1 Li1 87.8(7) 2_656 6_565 ?
Cl2 Li1 Li1 59.2(6) 1_554 6_565 ?
Cl2 Li1 Li1 51.9(5) 6_564 6_565 ?
Al1 Li1 Li1 58.4(5) 5_666 6_565 ?
Al3 Li1 Li1 59.4(5) . 6_565 ?
Na3 Li1 Na4 78.4(16) . 1_554 ?
O1 Li1 Na4 133.3(13) 5_666 1_554 ?
O3 Li1 Na4 130.7(10) 2_656 1_554 ?
O9 Li1 Na4 72.8(8) 2_656 1_554 ?
Cl2 Li1 Na4 56.4(6) 1_554 1_554 ?
Cl2 Li1 Na4 62.2(6) 6_564 1_554 ?
Al1 Li1 Na4 159.4(10) 5_666 1_554 ?
Al3 Li1 Na4 110.1(9) . 1_554 ?
Li1 Li1 Na4 106.1(6) 6_565 1_554 ?
Na3 Li1 Na2 84.7(15) . 1_554 ?
O1 Li1 Na2 129.1(11) 5_666 1_554 ?
O3 Li1 Na2 66.3(5) 2_656 1_554 ?
O9 Li1 Na2 137.4(9) 2_656 1_554 ?
Cl2 Li1 Na2 55.1(4) 1_554 1_554 ?
Cl2 Li1 Na2 60.6(4) 6_564 1_554 ?
Al1 Li1 Na2 103.6(7) 5_666 1_554 ?
Al3 Li1 Na2 160.8(10) . 1_554 ?
Li1 Li1 Na2 103.2(5) 6_565 1_554 ?
Na4 Li1 Na2 64.6(7) 1_554 1_554 ?
Na3 Li1 Na4 81.5(16) . 2_656 ?
O1 Li1 Na4 132.3(12) 5_666 2_656 ?
O3 Li1 Na4 127.3(9) 2_656 2_656 ?
O9 Li1 Na4 76.5(7) 2_656 2_656 ?
Cl2 Li1 Na4 52.0(5) 1_554 2_656 ?
Cl2 Li1 Na4 58.0(5) 6_564 2_656 ?
Al1 Li1 Na4 154.8(9) 5_666 2_656 ?
Al3 Li1 Na4 112.4(8) . 2_656 ?
Li1 Li1 Na4 103.4(5) 6_565 2_656 ?
Na4 Li1 Na4 4.8(7) 1_554 2_656 ?
Na2 Li1 Na4 61.0(6) 1_554 2_656 ?
Na4 Na4 O10 115(5) 2_657 2_657 ?
Na4 Na4 O15 111.2(18) 2_657 5_667 ?
O10 Na4 O15 76.4(8) 2_657 5_667 ?
Na4 Na4 Cl2 103(3) 2_657 . ?
O10 Na4 Cl2 125.2(6) 2_657 . ?
O15 Na4 Cl2 52.7(5) 5_667 . ?
Na4 Na4 O14 99(3) 2_657 3_556 ?
O10 Na4 O14 108.1(5) 2_657 3_556 ?
O15 Na4 O14 144.3(9) 5_667 3_556 ?
Cl2 Na4 O14 103.7(9) . 3_556 ?
Na4 Na4 O10 53(4) 2_657 . ?
O10 Na4 O10 153.6(6) 2_657 . ?
O15 Na4 O10 128.6(8) 5_667 . ?
Cl2 Na4 O10 81.1(7) . . ?
O14 Na4 O10 58.2(5) 3_556 . ?
Na4 Na4 O14 68(3) 2_657 4_556 ?
O10 Na4 O14 59.6(5) 2_657 4_556 ?
O15 Na4 O14 126.6(12) 5_667 4_556 ?
Cl2 Na4 O14 169.9(6) . 4_556 ?
O14 Na4 O14 81.6(4) 3_556 4_556 ?
O10 Na4 O14 94.7(4) . 4_556 ?
Na4 Na4 Cl2 65(3) 2_657 2_657 ?
O10 Na4 Cl2 83.0(8) 2_657 2_657 ?
O15 Na4 Cl2 49.1(6) 5_667 2_657 ?
Cl2 Na4 Cl2 78.3(4) . 2_657 ?
O14 Na4 Cl2 163.4(7) 3_556 2_657 ?
O10 Na4 Cl2 106.5(5) . 2_657 ?
O14 Na4 Cl2 94.2(7) 4_556 2_657 ?
Na4 Na4 O15 56.9(16) 2_657 . ?
O10 Na4 O15 130.0(9) 2_657 . ?
O15 Na4 O15 65.8(8) 5_667 . ?
Cl2 Na4 O15 48.2(5) . . ?
O14 Na4 O15 121.8(10) 3_556 . ?
O10 Na4 O15 66.7(6) . . ?
O14 Na4 O15 121.7(7) 4_556 . ?
Cl2 Na4 O15 47.7(5) 2_657 . ?
Na4 Na4 Cl2 101(3) 2_657 6_565 ?
O10 Na4 Cl2 122.8(6) 2_657 6_565 ?
O15 Na4 Cl2 48.9(5) 5_667 6_565 ?
Cl2 Na4 Cl2 4.6(2) . 6_565 ?
O14 Na4 Cl2 108.3(9) 3_556 6_565 ?
O10 Na4 Cl2 83.6(6) . 6_565 ?
O14 Na4 Cl2 166.7(7) 4_556 6_565 ?
Cl2 Na4 Cl2 73.8(3) 2_657 6_565 ?
O15 Na4 Cl2 45.7(5) . 6_565 ?
Na4 Na4 Na3 159(5) 2_657 1_556 ?
O10 Na4 Na3 85.9(5) 2_657 1_556 ?
O15 Na4 Na3 76.8(6) 5_667 1_556 ?
Cl2 Na4 Na3 65.9(4) . 1_556 ?
O14 Na4 Na3 68.5(5) 3_556 1_556 ?
O10 Na4 Na3 106.5(9) . 1_556 ?
O14 Na4 Na3 124.2(5) 4_556 1_556 ?
Cl2 Na4 Na3 125.8(5) 2_657 1_556 ?
O15 Na4 Na3 114.1(7) . 1_556 ?
Cl2 Na4 Na3 68.7(4) 6_565 1_556 ?
Na4 Na4 Li1 152(4) 2_657 1_556 ?
O10 Na4 Li1 91.2(6) 2_657 1_556 ?
O15 Na4 Li1 63.4(8) 5_667 1_556 ?
Cl2 Na4 Li1 51.3(6) . 1_556 ?
O14 Na4 Li1 81.0(8) 3_556 1_556 ?
O10 Na4 Li1 107.1(10) . 1_556 ?
O14 Na4 Li1 138.7(7) 4_556 1_556 ?
Cl2 Na4 Li1 111.7(6) 2_657 1_556 ?
O15 Na4 Li1 99.2(8) . 1_556 ?
Cl2 Na4 Li1 53.6(6) 6_565 1_556 ?
Na3 Na4 Li1 16.0(5) 1_556 1_556 ?
Cl2 Cl2 Li1 120.8(6) 6_565 1_556 ?
Cl2 Cl2 Na4 142.9(5) 6_565 . ?
Li1 Cl2 Na4 72.3(7) 1_556 . ?
Cl2 Cl2 Li1 51.9(5) 6_565 6_566 ?
Li1 Cl2 Li1 68.9(11) 1_556 6_566 ?
Na4 Cl2 Li1 126.1(6) . 6_566 ?
Cl2 Cl2 Na2 137.26(14) 6_565 . ?
Li1 Cl2 Na2 77.0(6) 1_556 . ?
Na4 Cl2 Na2 77.3(6) . . ?
Li1 Cl2 Na2 126.3(5) 6_566 . ?
Cl2 Cl2 Na4 137.6(4) 6_565 2_657 ?
Li1 Cl2 Na4 84.9(7) 1_556 2_657 ?
Na4 Cl2 Na4 12.8(6) . 2_657 ?
Li1 Cl2 Na4 136.1(7) 6_566 2_657 ?
Na2 Cl2 Na4 77.4(5) . 2_657 ?
Cl2 Cl2 Na4 32.5(5) 6_565 6_565 ?
Li1 Cl2 Na4 121.7(7) 1_556 6_565 ?
Na4 Cl2 Na4 110.4(10) . 6_565 ?
Li1 Cl2 Na4 64.3(6) 6_566 6_565 ?
Na2 Cl2 Na4 160.9(4) . 6_565 ?
Na4 Cl2 Na4 106.2(3) 2_657 6_565 ?
Cl2 Cl2 Na2 37.66(12) 6_565 6_565 ?
Li1 Cl2 Na2 122.8(6) 1_556 6_565 ?
Na4 Cl2 Na2 163.8(4) . 6_565 ?
Li1 Cl2 Na2 68.7(5) 6_566 6_565 ?
Na2 Cl2 Na2 99.60(15) . 6_565 ?
Na4 Cl2 Na2 151.1(3) 2_657 6_565 ?
Na4 Cl2 Na2 68.0(5) 6_565 6_565 ?
Cl2 Cl2 Na3 133.22(14) 6_565 1_556 ?
Li1 Cl2 Na3 12.4(6) 1_556 1_556 ?
Na4 Cl2 Na3 62.2(4) . 1_556 ?
Li1 Cl2 Na3 81.3(5) 6_566 1_556 ?
Na2 Cl2 Na3 68.66(19) . 1_556 ?
Na4 Cl2 Na3 74.4(3) 2_657 1_556 ?
Na4 Cl2 Na3 130.5(4) 6_565 1_556 ?
Na2 Cl2 Na3 131.85(16) 6_565 1_556 ?
Cl2 Cl2 Na4 37.6(4) 6_565 5_667 ?
Li1 Cl2 Na4 131.9(7) 1_556 5_667 ?
Na4 Cl2 Na4 106.5(3) . 5_667 ?
Li1 Cl2 Na4 75.6(6) 6_566 5_667 ?
Na2 Cl2 Na4 151.0(4) . 5_667 ?
Na4 Cl2 Na4 100.0(7) 2_657 5_667 ?
Na4 Cl2 Na4 11.6(5) 6_565 5_667 ?
Na2 Cl2 Na4 68.6(5) 6_565 5_667 ?
Na3 Cl2 Na4 139.2(4) 1_556 5_667 ?
Cl2 Cl2 Na3 41.84(12) 6_565 6_566 ?
Li1 Cl2 Na3 79.0(6) 1_556 6_566 ?
Na4 Cl2 Na3 131.9(5) . 6_566 ?
Li1 Cl2 Na3 10.1(5) 6_566 6_566 ?
Na2 Cl2 Na3 132.41(16) . 6_566 ?
Na4 Cl2 Na3 140.0(5) 2_657 6_566 ?
Na4 Cl2 Na3 55.7(3) 6_565 6_566 ?
Na2 Cl2 Na3 61.62(16) 6_565 6_566 ?
Na3 Cl2 Na3 91.38(16) 1_556 6_566 ?
Na4 Cl2 Na3 66.7(3) 5_667 6_566 ?
Na4 O15 Na4 123.1(11) 2_657 5_667 ?
Na4 O15 Na4 11.9(6) 2_657 . ?
Na4 O15 Na4 114.2(8) 5_667 . ?
Na4 O15 Na4 114.2(8) 2_657 6_565 ?
Na4 O15 Na4 11.9(6) 5_667 6_565 ?
Na4 O15 Na4 104.3(9) . 6_565 ?
Cu2 Cl1 Cu2 72.04(5) 6_565 . ?
Cu2 Cl1 Na1 126.68(7) 6_565 5_566 ?
Cu2 Cl1 Na1 74.08(4) . 5_566 ?
Cu2 Cl1 Na1 74.08(4) 6_565 1_554 ?
Cu2 Cl1 Na1 126.68(7) . 1_554 ?
Na1 Cl1 Na1 95.68(11) 5_566 1_554 ?
Cu2 Cl1 Na2 76.53(6) 6_565 2_656 ?
Cu2 Cl1 Na2 132.96(9) . 2_656 ?
Na1 Cl1 Na2 151.96(9) 5_566 2_656 ?
Na1 Cl1 Na2 74.33(7) 1_554 2_656 ?
Cu2 Cl1 Na2 132.96(9) 6_565 5_666 ?
Cu2 Cl1 Na2 76.53(6) . 5_666 ?
Na1 Cl1 Na2 74.33(7) 5_566 5_666 ?
Na1 Cl1 Na2 151.96(9) 1_554 5_666 ?
Na2 Cl1 Na2 102.08(13) 2_656 5_666 ?
Li1 O1 Li1 112.4(16) 2_656 5_666 ?
Li1 O1 Al1 101.4(8) 2_656 . ?
Li1 O1 Al1 101.4(8) 5_666 . ?
Li1 O1 Al3 103.4(8) 2_656 . ?
Li1 O1 Al3 103.4(8) 5_666 . ?
Al1 O1 Al3 134.5(3) . . ?
Li1 O1 Na3 13.0(8) 2_656 2_656 ?
Li1 O1 Na3 125.3(9) 5_666 2_656 ?
Al1 O1 Na3 98.37(17) . 2_656 ?
Al3 O1 Na3 97.48(17) . 2_656 ?
Li1 O1 Na3 125.3(9) 2_656 5_666 ?
Li1 O1 Na3 13.0(8) 5_666 5_666 ?
Al1 O1 Na3 98.37(17) . 5_666 ?
Al3 O1 Na3 97.48(17) . 5_666 ?
Na3 O1 Na3 138.2(3) 2_656 5_666 ?
Al2 O2 Al1 132.8(3) . . ?
Al2 O2 Cu2 102.01(19) . . ?
Al1 O2 Cu2 104.31(19) . . ?
Al2 O2 Cu2 102.01(19) . 6_565 ?
Al1 O2 Cu2 104.30(19) . 6_565 ?
Cu2 O2 Cu2 110.6(2) . 6_565 ?
P2 O3 Al1 130.4(2) . . ?
P2 O3 Li1 140.6(7) . 2_656 ?
Al1 O3 Li1 82.9(6) . 2_656 ?
P2 O3 Na3 122.1(2) . 2_656 ?
Al1 O3 Na3 95.35(18) . 2_656 ?
Li1 O3 Na3 19.6(6) 2_656 2_656 ?
P3 O4 Al1 129.4(2) . 5_666 ?
P3 O4 Cu2 133.5(2) . 5_666 ?
Al1 O4 Cu2 94.93(16) 5_666 5_666 ?
P2 O5 Al2 126.1(2) . . ?
P2 O5 Cu2 136.9(2) . 5_566 ?
Al2 O5 Cu2 91.92(15) . 5_566 ?
P2 O6 Cu4 117.6(2) . 8_465 ?
P2 O6 Na1 116.7(2) . . ?
Cu4 O6 Na1 112.85(17) 8_465 . ?
P2 O6 Na2 112.8(2) . 2_657 ?
Cu4 O6 Na2 104.64(17) 8_465 2_657 ?
Na1 O6 Na2 87.48(13) . 2_657 ?
P3 O7 Cu1 126.6(3) . 3 ?
P3 O7 Cu3 125.1(3) . 3 ?
Cu1 O7 Cu3 100.69(16) 3 3 ?
P3 O7 Na3 101.0(2) . . ?
Cu1 O7 Na3 100.90(18) 3 . ?
Cu3 O7 Na3 94.67(18) 3 . ?
P2 O8 Cu3 124.6(2) . 5_566 ?
P2 O8 Cu1 122.8(2) . 4_556 ?
Cu3 O8 Cu1 95.23(15) 5_566 4_556 ?
P3 O9 Al3 135.1(2) . . ?
P3 O9 Li1 137.1(7) . 2_656 ?
Al3 O9 Li1 85.3(6) . 2_656 ?
P3 O9 Na3 119.4(2) . 2_656 ?
Al3 O9 Na3 98.23(19) . 2_656 ?
Li1 O9 Na3 20.3(6) 2_656 2_656 ?
P3 O10 Cu4 114.4(2) . . ?
P3 O10 Na4 115.9(4) . 2_657 ?
Cu4 O10 Na4 96.7(3) . 2_657 ?
P3 O10 Na2 127.9(2) . . ?
Cu4 O10 Na2 104.20(17) . . ?
Na4 O10 Na2 91.5(5) 2_657 . ?
P3 O10 Na4 127.0(4) . . ?
Cu4 O10 Na4 95.2(3) . . ?
Na4 O10 Na4 12.3(9) 2_657 . ?
Na2 O10 Na4 80.0(4) . . ?
P1 O11 Cu1 130.6(2) . . ?
P1 O11 Cu4 118.4(2) . 5_666 ?
Cu1 O11 Cu4 105.08(18) . 5_666 ?
P1 O11 Na3 80.98(19) . 3_445 ?
Cu1 O11 Na3 93.75(17) . 3_445 ?
Cu4 O11 Na3 124.32(18) 5_666 3_445 ?
P1 O12 Cu3 129.9(3) . . ?
P1 O12 Cu4 121.4(2) . 4_546 ?
Cu3 O12 Cu4 103.15(19) . 4_546 ?
P1 O12 Na3 85.3(2) . 3_445 ?
Cu3 O12 Na3 93.02(18) . 3_445 ?
Cu4 O12 Na3 118.6(2) 4_546 3_445 ?
P1 O13 Cu2 128.1(2) . . ?
P1 O13 Na1 118.7(2) . 5_566 ?
Cu2 O13 Na1 98.49(17) . 5_566 ?
P1 O13 Na2 115.0(2) . 5_666 ?
Cu2 O13 Na2 101.15(17) . 5_666 ?
Na1 O13 Na2 86.49(13) 5_566 5_666 ?
P1 O14 Cu4 139.9(3) . 3_444 ?
P1 O14 Na4 113.7(5) . 3_444 ?
Cu4 O14 Na4 95.7(4) 3_444 3_444 ?
P1 O14 Na2 119.7(3) . 3_444 ?
Cu4 O14 Na2 92.12(19) 3_444 3_444 ?
Na4 O14 Na2 77.0(5) 3_444 3_444 ?
P1 O14 Na4 125.0(5) . 4_546 ?
Cu4 O14 Na4 82.7(4) 3_444 4_546 ?
Na4 O14 Na4 13.1(6) 3_444 4_546 ?
Na2 O14 Na4 77.7(5) 3_444 4_546 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 O11 1.957(4) 7_556 ?
Cu1 O11 1.958(4) . ?
Cu1 O7 2.118(4) 5_666 ?
Cu1 O7 2.118(4) 3_445 ?
Cu1 O8 2.308(4) 6_565 ?
Cu1 O8 2.308(4) 4_546 ?
Cu1 Na3 3.471(4) 3_445 ?
Cu1 Na3 3.471(4) 5_666 ?
Cu2 O13 1.886(3) . ?
Cu2 O2 1.918(3) . ?
Cu2 O4 2.027(4) 5_666 ?
Cu2 O5 2.048(4) 5_566 ?
Cu2 Cl1 2.6815(15) . ?
Cu2 Al2 2.8752(6) . ?
Cu2 Al1 2.951(2) . ?
Cu2 Na1 3.2770(8) 5_566 ?
Cu2 Na2 3.381(3) 5_666 ?
Cu3 O12 2.002(5) 2_556 ?
Cu3 O12 2.002(5) . ?
Cu3 O8 2.208(4) 6_565 ?
Cu3 O8 2.208(4) 5_566 ?
Cu3 O7 2.214(5) 4_546 ?
Cu3 O7 2.214(4) 3_445 ?
Cu3 Na3 3.379(4) 3_445 ?
Cu3 Na3 3.379(4) 4_546 ?
Cu4 O10 1.891(4) . ?
Cu4 O6 1.896(3) 8_565 ?
Cu4 O14 1.999(4) 3_556 ?
Cu4 O12 2.301(4) 4_556 ?
Cu4 O11 2.302(4) 5_666 ?
Cu4 Na4 3.198(18) 2_657 ?
Cu4 Na2 3.401(3) . ?
Cu4 Na4 3.427(18) . ?
Cu4 Na2 3.443(3) 7_667 ?
Cu4 Na1 3.592(3) 7_567 ?
P1 O14 1.500(4) . ?
P1 O13 1.541(4) . ?
P1 O12 1.546(4) . ?
P1 O11 1.549(4) . ?
P1 Na3 2.930(4) 3_445 ?
P1 Na2 3.415(3) 5_666 ?
P1 Na1 3.433(3) 5_566 ?
P2 O8 1.524(4) . ?
P2 O3 1.533(4) . ?
P2 O6 1.542(3) . ?
P2 O5 1.559(4) . ?
P2 Na2 3.349(3) 2_657 ?
P2 Na1 3.3877(12) . ?
P3 O9 1.513(4) . ?
P3 O10 1.531(4) . ?
P3 O7 1.535(4) . ?
P3 O4 1.543(4) . ?
P3 Na3 3.067(4) . ?
P3 Na4 3.33(2) 2_657 ?
P3 Na3 3.368(4) 2_656 ?
Al1 O1 1.812(6) . ?
Al1 O2 1.818(6) . ?
Al1 O3 1.878(4) 6_565 ?
Al1 O3 1.878(4) . ?
Al1 O4 1.978(4) 5_666 ?
Al1 O4 1.978(4) 2_656 ?
Al1 Li1 2.74(2) 2_656 ?
Al1 Li1 2.74(2) 5_666 ?
Al1 Na3 3.213(4) 2_656 ?
Al1 Na3 3.213(4) 5_666 ?
Al2 O2 1.780(5) . ?
Al2 O2 1.780(5) 5_566 ?
Al2 O5 1.950(4) . ?
Al2 O5 1.950(4) 5_566 ?
Al2 O5 1.950(4) 6_565 ?
Al2 O5 1.950(4) 2_556 ?
Al3 O1 1.864(5) 5_666 ?
Al3 O1 1.864(5) . ?
Al3 O9 1.891(4) 5_666 ?
Al3 O9 1.891(4) 6_565 ?
Al3 O9 1.891(4) 2_656 ?
Al3 O9 1.891(4) . ?
Al3 Li1 2.82(2) 6_565 ?
Al3 Li1 2.82(2) 2_656 ?
Al3 Li1 2.82(2) 5_666 ?
Al3 Li1 2.82(2) . ?
Al3 Na3 3.226(4) . ?
Al3 Na3 3.226(4) 2_656 ?
Na1 O6 2.402(4) . ?
Na1 O6 2.402(4) 2_557 ?
Na1 O13 2.416(4) 6_566 ?
Na1 O13 2.416(4) 5_566 ?
Na1 Cl1 2.758(3) 5_566 ?
Na1 Cl1 2.758(3) 1_556 ?
Na1 Na2 3.344(2) 2_657 ?
Na1 Na2 3.344(2) 1_455 ?
Na2 O10 2.400(4) . ?
Na2 O6 2.434(4) 2_657 ?
Na2 O13 2.464(4) 5_666 ?
Na2 Cl2 2.676(7) . ?
Na2 O14 2.678(6) 3_556 ?
Na2 Cl1 2.777(3) 5_666 ?
Na2 Cl2 2.972(7) 6_565 ?
Na2 Li1 3.18(2) 1_556 ?
Na2 Na3 3.208(5) 1_556 ?
Na2 Na4 3.28(3) . ?
Na3 Li1 0.82(3) . ?
Na3 O9 2.357(6) 2_656 ?
Na3 O7 2.378(6) . ?
Na3 O1 2.402(4) 5_666 ?
Na3 O3 2.437(6) 2_656 ?
Na3 O12 2.618(6) 3 ?
Na3 O11 2.741(6) 3 ?
Na3 Na4 2.902(18) 1_554 ?
Na3 Cl2 2.994(7) 1_554 ?
Li1 O1 1.72(2) 5_666 ?
Li1 O3 2.24(2) 2_656 ?
Li1 O9 2.25(2) 2_656 ?
Li1 Cl2 2.42(2) 1_554 ?
Li1 Cl2 2.64(2) 6_564 ?
Li1 Li1 2.87(5) 6_565 ?
Li1 Na4 2.95(3) 1_554 ?
Li1 Na4 3.53(3) 2_656 ?
Na4 Na4 0.63(3) 2_657 ?
Na4 O10 2.37(2) 2_657 ?
Na4 O15 2.561(17) 5_667 ?
Na4 Cl2 2.581(18) . ?
Na4 O14 2.59(2) 3_556 ?
Na4 O10 2.69(2) . ?
Na4 O14 2.764(19) 4_556 ?
Na4 Cl2 2.788(19) 2_657 ?
Na4 O15 2.851(18) . ?
Na4 Cl2 2.899(17) 6_565 ?
Cl2 Cl2 0.387(16) 6_565 ?

_cod_database_fobs_code 2109099
